27 Mar 2019 - The particles show a regular spherical shape with an average diameter of 15 Â± 10 Î¼m, measured by scanning electron microscopy (SEM) ...
Publication Date (Web): August 10, 2018 ... Additionally, we demonstrate the ability to create well-adhering 100% reflective coatings by coating double layers ...
Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, the ... Normal University, Guangzhou Higher Education Mega Center, 510006, ...
Additionally, we demonstrate the ability to create well-adhering ~100% reflective ..... reflecting coatings, which are suitable for smart window applications. This.
Aug 10, 2018 - From Chaos to Order: Evaporative Assembly and Collective Behavior in Drying Liquid Crystal Droplets. The Journal of Physical Chemistry ...
15 hours ago - ... oC higher than that of the white nano SiO2 coating. Furthermore, the NIR reflective coating exhibited a typical SH property due to its low surface energy and high surface roughness, which may allow for self-cleaning performance in
Apr 23, 2018 - Recently, infrared reflective pigments possessing deep colors have attracted much attention. However, in polluted air, the coatings consisting of ...
Apr 23, 2018 - (10) A lot of manpower and energy are required to clean the ... (15) Zhu et al. prepared a superhydrophilic, anti-infrared, self-cleaning coating using a two-layer structure of SiO2 (top)/TiO2 (bottom) .... Among all solar energy, infr
Dec 26, 2016 - In total, compared to F-free, â¼1, â¼2, and â¼7 wt % F doped MNRs, â¼5 wt % F doped MNR significantly enhanced antibacterial and osteogenic activities, especially new bone formation and osseointegration in the bacteria-infected cas
Dec 26, 2016 - ... and Osteogenic Activities of Bone Implants in Bacteria-Infected Cases ... bone formation and osseointegration in the bacteria-infected case, ...
Subscriber access provided by UNIV OF LOUISIANA
Applications of Polymer, Composite, and Coating Materials
Patterned full-color reflective coatings based on photonic cholesteric liquid-crystalline particles Alberto Belmonte, Tom Bus, Dirk J. Broer, and Albert P. H. J. Schenning ACS Appl. Mater. Interfaces, Just Accepted Manuscript • DOI: 10.1021/acsami.9b02680 • Publication Date (Web): 27 Mar 2019 Downloaded from http://pubs.acs.org on March 28, 2019
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Patterned full-color reflective coatings based on photonic cholesteric liquid-crystalline particles Alberto Belmonte1,3 Tom Bus1,3 Dirk J. Broer1,2,3 and Albert P.H.J. Schenning1,2,3,*
1) Stimuli-responsive Functional Materials and Devices, Department of Chemical Engineering, Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, The Netherlands 2) SCNU-TUE Joint Laboratory of Device Integrated Responsive Materials (DIRM), South China Normal University, Guangzhou Higher Education Mega Center, 510006, Guangzhou, China 3) Institute for Complex Molecular Systems, Eindhoven University of Technology, Den Dolech 2, 5600 MB, Eindhoven, The Netherlands * Corresponding author, e-mail: [email protected]
Abstract An easy approach to pattern angular-independent, multi-color reflective coatings based on cholesteric liquid crystalline (CLC) particles is presented. CLC particles are fabricated by emulsification, which is a scalable, cost-effective and environmentally-friendly synthesis process. The photonic particles can be easily dispersed in a binder to produce reflective coatings. Furthermore, a simple strategy to remove the photonic cross-communication between the particles has been developed. By incorporating a reactive blue/green absorbing dye into the network structure of the CLC particles the cross-communication is absorbed by the dye leading to well-defined structural colors. Moreover, we demonstrate the possibility of producing patterned multi-color images by controlled swelling of the particles by the binder.
Introduction In the field of optical materials, photonic crystals (PhCs) and polymers are typically used for applications such as optical sensors1,2, displays3,4 and reflective coatings5–7. PhCs are used because they can modulate incident light with specific wavelengths to generate bright reflected structural colors. PhCs consist of one-, two- or three-dimensional, periodic nano-structured materials, having alternating refractive indices. Self-assembled colloidal structures8 or spherical colloidal clusters9 are an example of photonic crystals that have bright structural colors due to their sub-micrometer three dimensional organization10. Despite the recent progress in PhCs11, the assembling of such an ordered periodical structure still involves in most cases complex and time-consuming steps. For instance, multi-step lithographic techniques, which are often used in this regard, limit the final design and increase the cost. In contrast to PhCs, cholesteric liquid crystals (CLC) are soft photonic polymers that exhibit selective light reflection due to the presence of a helical molecular organization12. The reflected wavelength depends on the pitch of the helical structure which can be easily tuned by chemical composition, temperature or other external stimuli13,14, and can be stabilized by chemical crosslinking (i.e. by using acrylate-based liquid crystal monomers)15,16. The CLC alignment, which is crucial for proper reflection of light of a specific wavelength, requires the use of alignment layers. In addition, CLC-based reflective materials have a pseudo one-dimensional organization, leading to incident-angular-dependent reflection according to Bragg’s law. To this end, it remains a challenge to 2 ACS Paragon Plus Environment
develop a facile method to prepare patterned multi-color photonic materials with angularindependent reflective properties. To meet this challenge, three-dimensional organization of the helical structure by means of CLC polymer particles can be used to fabricate the angular-independent reflective materials17–23. Such CLC particles can be easily processed and do not require alignment layers. Furthermore, they exhibit controlled expansion-contraction effects by solvent-swelling with large color-shifts3,24. In a recent work, Beltran et. al25 show a versatile approach to produce blue angular-independent reflective films based on CLC particles synthesized by suspension polymerization using organic solvents. In another research study, Lee et. al26 fabricated green reflective elastic films based on elastomeric reconfigurable CLC micro-capsules. Nevertheless, the problem remains that the color of CLC particles-based coatings is, in most of the cases, influenced by the well-known photonic crosscommunication phenomenon27. This phenomenon occurs when off-normal incident light is reflected from one particle at a specific angle that can be reflected back to the observer by the neighboring particles, leading to multiple wavelengths reaching the observer17,27,28. This is a clear disadvantage when green and red colors are intended, as blue light also reaches the observer. Because of this, patterned and/or full-color reflective coatings based on photonic cholesteric liquid-crystalline particles have not been reported in the literature to date. In this work we present a simple and effective method to fabricate angular-independent, patterned, reflective coatings based on photonic cholesteric liquid-crystalline particles. For the synthesis of the CLC particles, we used the suspension polymerization, because it is consistent and allows large-scale production of particles in water25,29. To minimize photonic cross-communication between the CLC particles, we added a reactive blue/green absorbing dye to the CLC mixture. By using this costeffective and environmentally-friendly water-based emulsification process, we photo-polymerized the CLC droplets into polymer particles. After the CLC particles were dispersed in a binder, we were able to fabricate reflective coatings with pure structural color reflection by simple coating techniques
that do not require alignment layers. Moreover, we fabricated bicolor arbitrary patterns by controlled absorption of the binder.
Results and discussion In order to synthesize the multicolor photonic particles, we used a CLC mixture containing reactive monomers (RM1 and RM2), non-reactive monomer (NRM), photo-initiator Irgacure 819 and thermalinhibitor (2,6-Di-tert-butyl-4-methylphenol) (Figure 1a). The nomenclature and composition for all the formulations of the study is detailed in Table S1. We selected NRM as chiral dopant (HTP ≈ 7.230) because it helps to decrease the cholesteric temperature window to room temperature as can be deduced from the calorimetric analyses (Figure S1a). Furthermore, NRM acts as a porogen and by changing its concentration from 20% to 40%, the near-infrared reflection band shifts to the blue region of the visible spectrum as evidenced by the UV-Vis-NIR spectra (Figure S1b). Finally, we chosen RM1 and RM2 reactive monomers to fix the CLC alignment and build-up a crosslinked network with a glass transition temperature (Tg) around 55°C as deduced from the calorimetric analyses in Figure S2.
Figure 1. Synthesis and characterization of the CLC particles: a) compounds and scheme of the synthesis process, b) Scanning Electron Microscopy (SEM) image of the particles and c) Transmission Electron Microscopy (TEM) image of the cross-section of a particle and Polarized Optical Microscopy (POM) image of large-pitch particle including an illustration of the monomers orientation in the cholesteric layers. We used suspension polymerization to synthesize the CLC particles, because it is a suitable method for large-scale production of particles. The method makes use of a water-based continuous phase with polyvinylpyrrolidone (PVP) as surfactant (Figure 1a). Monomer droplets were obtained after high-speed stirring for 15 minutes at T > Tiso and the cholesteric alignment was further induced on cooling down to room temperature (1 in Figure 1a). After photo-polymerization (2 in Figure 1a) and further extraction of NRM (3 in Figure 1a) porous CLC polymer particles were obtained. The yield of particles was around 65%. In Figure S3, the IR spectra reveal the disappearance of the stretching vibration at 1630 cm-1 (stretching C=C), indicating that all acrylate groups have reacted. We confirmed the extraction of NRM by the disappearance of the C≡N stretching peak at 2260-2220 cm1.
The particles show a regular spherical shape with an average diameter of 15 ± 10 µm, measured by
scanning electron microscopy (SEM) (Figure 1b). The cholesteric layers in the spherical particles follow a radial alignment as deduced from the existence of concentric circles in the transmission 5 ACS Paragon Plus Environment
electron microscopy (TEM) image of the cross-section of a particle in Figure 1c. In order to analyze the cholesteric layers under polarized optical microscopy (POM), we synthesized particles with a large-pitch of 1.5 µm by using the far-IR mixture (Figure 1c). The image confirms radial stacking of the cholesteric layers in concentric rings. Moreover, the presence of a radial defect line suggests that the alignment follows the well-known Frank-Pryce model. In this model, the orientation of the monomers in each cholesteric layer draw a family of circles corresponding to the intersection of all planes passing through the same point as illustrated in Figure 1c31. This alignment is attributed to the use of PVP as surfactant, which reduces the energy at the water/droplet interface. Low interface energy favors planar alignment of the monomers and enables the growing of the helical structure towards the center.
Figure 2. POM images of single blue, green and red particles in poly(methylphenyl)siloxane as indexmatching immersion oil (n = 1.53) and a schematic picture of the alignment of the helical structure within the photonic particles.
In Figure 2, we show POM images of isolated particles dispersed in refractive index matching matrix (poly(methylphenyl)siloxane, PMPS, refractive index ≈ 1.53). The nomenclature of the particles is detailed in Table S1. The particles show the well-known Maltese-cross when observed between crossed-polarizers, which confirms the radial growing of the helical structure. 6 ACS Paragon Plus Environment
presence of a defect line when observed without crossed-polarizers confirms the Frank-Pryce model for the particles reflecting in the visible region of the spectrum (i.e. in the red particle). When observed in reflection mode a bright spot appears at the center of the particles. This is attributed to the Bragg reflection of the particles which is angular-independent for the observer. As stated in the introduction, only incident light reflected into the plane normal to the observer comes back to the observer as illustrated in Figure 2. In Figure 1c we showed the TEM image of the cross-section of a red particle. The distance measured between three consecutive circles of the same tonality defines the helical pitch when the cut goes throughout the center of the particle. Then, on applying the relation:
, where θ is the viewing angle,
is the average refractive index and P is the
pitch of the helical structure, the Bragg reflection, λ0°, can be calculated. When assuming a typical value of
= 1.6 for LC particles, the calculated λ0° is around 645 nm, which matches with the
observed red dot of the red particle. It must be noted that the Bragg reflection of the polymer particles is blue-shifted from the expected structural color according to the UV-Vis spectra of the CLC mixtures (Figure S1b). This is explained by the inherent shrinkage of the particles caused by the extraction of NRM during the synthesis process (step 3, Figure 1a).
Figure 3. a) Pictures of 70µm coatings made with blue, green and red particles, respectively, including the POM image of the red coating b) UV-Vis spectra of the coatings (dashed line indicates the reflection band of the red particles) and c) photonic cross-communication between particle arrays.
The preparation of CLC particle based reflective coatings requires a transparent, refractive index matching binder. We used a commercial high refractive index (n ≈ 1.57) photo-curable monomer, AgiSynDSM 2871. To fabricate thin coatings, we spread a dispersion of 40% in weight of polymer particles in the binder between glass plates. After photo-polymerization of the binder, different coatings were obtained having blue, green and red particles, respectively (Figure 3a). The coating made of blue particles clearly shows a dark blue color according to the particles’ Bragg reflection; in contrast, coatings made of green and red particles both deviate from their expected colors. The coating made of green particles has a light blue color, whereas the coating made of red particles is almost completely white. To better understand the deviation of the color observed with the color expected, we measured UV-Vis spectra of the coatings (Figure 3b). The coating made of blue particles shows a single reflection peak centered at 460nm in agreement with the observed color. In contrast, coatings made of green and red particles show a double peak reflection. The red-shifted peak is 8 ACS Paragon Plus Environment
attributed to the Bragg reflection of the particles, because it matches with the observed colors in Figure 2, while the broader, blue-shifted peak is attributed to the photonic cross-communication. Photonic cross-communication takes place when incident light non-orthogonal to the cholesteric plane is reflected towards neighboring particles and these particles reflect it back to the observer. Total internal reflection can also occur at the binder/air interface leading to complex communication patterns. The broad peak associated to cross-communication extends to the UV region explaining the whitish color for the “red” coating and the bluish color for the “green” coating. Note that crosscommunication of blue particles is not visible to the naked eye because it is shifted to the UV region. To further understand the cross-communication phenomenon, we have analyzed a thin film of NearIR particles (λ0° = 796 nm) dispersed in the refractive index matching siloxane, PMPS, under the optical microscope (Figure 3c). Close to the center of the particles we can observe (F1) directcommunication (DC) as multiple green rays pointing towards neighboring particles. On focusing towards the top of the particle (F2-F3), DC rays vanish and green-reddish bright dots appear closer to the center of the particle in the x-y plane. This is caused by total internal reflection (TIR) of the light reflected from one particle to the PMPS/air interface and reflected back to the observer by neighboring particles. In general, we observe green DC rays and red TIR dots suggesting that DC takes place around 45° (λ45° = 562 nm) and TIR around 30° (λ30° = 562 nm) regardless of the particles size (a detailed explanation is provided in the Supporting Information, Figure S4). Finally, we observe two concentric green and red reflection rings appearing at a certain distance from the center of most of the particles. This can be related to self-communication (SC) with the air interface, which occurs when the light is self-reflected from the PMPS/air interface to the particle and reflected back to the observer, as depicted in Figure S4b. As can be seen, SC leads to bright blue, green and red reflection which explains the strong communication peaks observed in the UV-Vis spectra and the bluegreenish reflection surrounding the particles in the POM image of Figure 3a.
Figure 4. a) Scheme of the photonic cross-communication absorption mechanism by adding a blue /green-absorbing dye acrylate (DR1A) to the polymer particles and b) photographs of 70 µm coatings made of red, green and blue particles with and without DR1A and the corresponding UV-Vis spectra.
In order to minimize the effect of the photonic cross-communication we added a small amount (0.1% in weight) of a reactive dye (DR1A) to the CLC mixtures before the suspension polymerization (Figure 1a). The dye has an absorption peak between 450 to 600 nm (Figure S5) and therefore, is expected to absorb cross-communicating rays (Figure 4a). Coatings made of red, green and blue DR1A-photonic particles were prepared as described before and the UV-Vis spectra were measured (Figure 4b). The coating made of green DR1A-particles shows clearly a green-yellowish color and the coating made of red DR1A-particles has a reddish color according to the Bragg reflection wavelength. Both spectra reveal a strong decrease in the reflection band at the absorption region of the dye, suggesting that the dye is effectively absorbing the blue and green cross-communication. Note that the use of 0.1% in weight of DR1A is enough to minimize the cross-communication while maintaining 80% transmission in the absorption region of the dye (Figure S5). It must be noted that the use of DR1A
for blue reflective coatings is not appropriate since the dye absorbs in the green region and therefore the blue turns into purple as it is observed. Regardless, the blue reflective coatings do not show cross-communication in the visible region, hence the dye is not required to achieve proper coloration.
Figure 5. a) Blue, green, yellowish and red coatings shown at different angles (top) and zoom in of the coatings (bottom) and b) bicolor patterned reflective coating made by using blue DR1A-particles and a photo-mask. By using different structural colored particles containing DR1A, we were able to fabricate reflective coatings that exhibit angular-independent structural colors when observed by the naked eye (Figure 5a). Additionally, we show the possibility of tuning the reflected color from the same batch of particles by altering the absorption of the binder. Swelling of the particles leads to an increase of the pitch and, therefore, a red-shift of the reflected color. This can be used to prepare patterned images (Figure 5b). We fabricated a patterned bicolored, purple and green, image by using blue DR1Aparticles. First, we spread a dispersion of 40% in weight of polymer particles in the binder between glass plates. Then, we placed a photomask patterned with the tree-model on top of the sandwich and the visible region was exposed to UV. In the exposed region the binder was polymerized and the particles were immobilized. Afterwards, we raised up the temperature above the Tg of the particles 11 ACS Paragon Plus Environment
(Tg ≈ 55°C) and a red-shift was observed in the unexposed regions, demonstrating the absorption of the unreacted acrylates by the flexible porous particles. We carried out a second UV-curing process to the entire sample and the result reveals a bicolor image with defined contours. In certain areas, both left and right sides, and around the tree crown, a bluish color is observed instead of green. This is attributed to an insufficient amount of binder to achieve the maximum swelling of the particles. During the heating process, the viscosity of the binder decreases and therefore uncontrolled flow driven by thickness irregularities in between the glass plates may take place. It is worth noting that by decreasing the crosslinking density of the particles, that is decreasing the RM1 to RM2 relation (Figure 1a), we expect an enhancement of the swelling capabilities due to an increased flexibility of the network structure and therefore a larger color change, for instance, from blue to red.
Conclusions An easy and effective approach for the preparation of angular-independent full-color reflective coatings based on CLC particles is shown. The particles are synthesized following a scalable, costeffective and environmentally-friendly process. The optical properties of the particles are easily controlled by the amount of chiral dopant in the CLC mixture. Particles from UV to IR reflection can be synthesized and easily dispersed in a binder to further prepare reflective coatings by simple coating techniques. The optical properties of the coatings have been extensively discussed including relevant insights to the photonic cross-communication phenomenon between particles and the surrounding medium. It has been suggested that not only direct-communication or total internal reflection can reach the observer, but also self-communication with the surrounding results in light to the observer. Thanks to the addition of a reactive blue/green absorbing dye the green and blue photonic-communication is absorbed, allowing the preparation of reflective coatings with reflections ranging from blue to red with accurate control on the final color. In addition, a bicolor patterned
image has been prepared from a single batch of particles owing to the swelling properties of the porous structure above the glass transition temperature.
CLC particles synthesis:
The CLC particles were synthesized by suspension polymerization (see scheme in Figure 1a). The monomer mixture consists of reactive mesogens RM1 (monoacrylate), RM2 (crosslinker diacrylate) and a non-reactive chiral dopant NRM, all of them purchased from Merck. Photo-initiator Irgacure® 819 (1%wt) was purchased from CIBA Inc. and thermal-inhibitor (2,6-di-tert-butyl-4-methylphenol, BHT, 0.5%wt) was purchased from Sigma-Aldrich. All compounds were used without any further purification. The aqueous phase was formed by dissolving polyvinylpyrrolidone (PVP, Mw = 40k, Sigma Aldrich) in deionized water (1 mM). The synthesis was carried out in three steps: the formation of the CLC droplets (emulsification), the polymerization and the extraction of the non-reactive monomer (NRM). For the emulsification, the monomers mixture, photo-initiator and thermalinhibitor were first dissolved in dichloromethane and sonicated for 3 minutes. Then, the solvent was flushed with air and completely evaporated by raising the temperature up to 80°C during 10 minutes. Afterwards, the preheated aqueous phase at 80°C was poured on the melted monomers and the droplets were formed and stabilized by stirring with an IKA® WERKE (Ultra-Turrax T8) at 15.000 rpm for 15 minutes. Finally, the cholesteric alignment was induced by slowly cooling down the emulsion to room temperature. For the polymerization, the emulsion was poured in a thin glass container placed inside a nitrogen box with continuous magnetic stirring (300 rpm). The polymerization was triggered by shinning UV light at maximum intensity with a mercury lamp (EXFO Omnicure S2000, λ = 350 – 450 nm) for 30 minutes to ensure full conversion of the acrylate groups. Note that the thin glass container helps the UV light to cross throughout the sample. Once the polymerization is over, 13 ACS Paragon Plus Environment
the particles were washed first with ethanol to remove the surfactant and then twice with tetrahydrofuran to extract the NRM monomer.
Particles-based coatings were prepared by dispersing the particles in a commercial photo-curable monomer, AgiSynDSM 2871 (O-phenylphenoxyethyl acrylate mixture), with refractive index matching the refractive index of the particles (n = 1.571) and transparency in the visible region. One drop of the dispersion was poured on the center of a clean glass plate and four small droplets of a dispersion of 70µm particles in photo-curable resin were added to the corners of the plate as spacers. Then, a second clean glass plate was carefully placed on top and slightly compressed following regular circular movements until the 70µm particles are in contact with both glass plates. Finally, the cell was exposed to UV light for five minutes in order to polymerize the acrylates. The coatings were left in between glass plates for the further measurements.
Thermal transitions of the liquid-crystalline mixtures and the particles were analyzed by differential scanning calorimetry (DSC) using a TA Instruments Q2000 calorimeter with constant heating and cooling rates of 10°C/min. Optical images of the cholesteric phases were taken by polarized optical microscopy (POM) using a microscope (Leica DM2700M) equipped with a Leica MC170 HD highresolution camera in reflection mode under crossed-polarizers. The conversion of the acrylate groups and the extraction of the NRM monomer were studied by infrared spectroscopy using a Varian 670 IR spectrometer equipped with a microscopy setup over a range of 4000-650 cm-1. POM images of the particles were taken in reflection and transmission mode either under crossed- or without polarizers. The particles size population was analyzed by scanning electron microscopy (SEM) using a JEOL SEM JSM-IT100: particles were dispersed in sticky conductive film and sputter-coated with a gold target at 14 ACS Paragon Plus Environment
60 mA during 30 seconds. The internal configuration of the cholesteric layers was analyzed by transmission electron microscopy (TEM) of the particles cross-section using a Tecnai 20 (type Sphera) by FEI operating with a LaB6 filament at 200 kV under slight under focus conditions. Particles were embedded in an EPOFIX epoxy media. Cross-sections were cut at room temperature using an ultramicrotome (Reichert-Jung Ultracut E) with 60 nm setting thickness. The obtained cross-sections were transferred to a carbon film covered grid (Electron Microscopy Sciences, CF200-CU). The reflection of the CLC mixtures and particles-based coatings was measured through ultraviolet-visible spectroscopy (UV-Vis) by using a Perkin Elmer Lambda 750 with a 150 mm integrating sphere over a range of 2501000 nm (wavelength) at room temperature.
Composition of the CLC mixtures. DSC curves, UV-Vis and FTIR spectra of the CLC mixtures and particles. Photonic cross-communication pictures and explanation. Transmission spectra of the DR1A dissolved in the binder.
This work was financially supported by the Netherlands Organization for Scientific Research (TOPPUNT 718.016.003). The authors thank Audrey Debije-Popson and Michael Debije for valuable comments on the manuscript.
Mulder, D. J.; Schenning, A. P. H. J.; Bastiaansen, C. W. M. Chiral-Nematic Liquid Crystals as One Dimensional Photonic Materials in Optical Sensors. J. Mater. Chem. C 2014, 2 (33), 6695– 6705.
Davies, D. J. D.; Vaccaro, A. R.; Morris, S. M.; Herzer, N.; Schenning, A. P. H. J.; Bastiaansen, C. W. M. A Printable Optical Time-Temperature Integrator Based on Shape Memory in a Chiral Nematic Polymer Network. Adv. Funct. Mater. 2013, 23 (21), 2723–2727.
Ha, N. Y.; Ohtsuka, Y.; Jeong, S. M.; Nishimura, S.; Suzaki, G.; Takanishi, Y.; Ishikawa, K.; Takezoe, H. Fabrication of a Simultaneous Red-Green-Blue Reflector Using Single-Pitched Cholesteric Liquid Crystals. Nat. Mater. 2008, 7 (1), 43–47.
Arsenault, A. C.; Puzzo, D. P.; Manners, I.; Ozin, G. A. Photonic-Crystal Full-Colour Displays. Nat. Photonics 2007, 1 (8), 468–472.
Khandelwal, H.; Schenning, A. P. H. J.; Debije, M. G. Infrared Regulating Smart Window Based on Organic Materials. Adv. Energy Mater. 2017, 7 (14).
Moirangthem, M.; Schenning, A. P. H. J. Full Color Camouflage in a Printable Photonic BlueColored Polymer. ACS Appl. Mater. Interfaces 2018, 10 (4), 4168–4172.
Heeswijk, E. P. A. V.; Kloos, J. J. H.; Heer, J. De; Hoeks, T.; Grossiord, N.; Schenning, A. P. H. J. Well-Adhering, Easily Producible Photonic Reflective Coatings for Plastic Substrates. ACS Appl. Mater. Interfaces 2018, 10 (35), 30008–30013.
Lee, I.; Kim, D.; Kal, J.; Baek, H.; Kwak, D.; Go, D.; Kim, E.; Kang, C.; Chung, J.; Jang, Y.; et al. Quasi-Amorphous Colloidal Structures for Electrically Tunable Full-Color Photonic Pixels with Angle-Independency. Adv. Mater. 2010, 22 (44), 4973–4977.
Lopez-Leon, T.; Fernandez-Nieves, A. Drops and Shells of Liquid Crystal. Colloid Polym. Sci. 2011, 289 (4), 345–359.
Chen, L.; Li, Y.; Fan, J.; Bisoyi, H. K.; Weitz, D. A.; Li, Q. Photoresponsive Monodisperse Cholesteric Liquid Crystalline Microshells for Tunable Omnidirectional Lasing Enabled by a Visible Light-Driven Chiral Molecular Switch. Adv. Opt. Mater. 2014, 2 (9), 845–848.
Bisoyi, H. K.; Bunning, T. J.; Fan, J.; Li, Q.; Zola, R. S.; Yang, D.; Weitz, D. A.; Li, Y. Light-Directing Omnidirectional Circularly Polarized Reflection from Liquid-Crystal Droplets. Angew. Chemie Int. Ed. 2014, 54 (7), 2160–2164.
Wang, L.; Chen, D.; Gutierrez-Cuevas, K. G.; Krishna Bisoyi, H.; Fan, J.; Zola, R. S.; Li, G.; Urbas, A. M.; Bunning, T. J.; Weitz, D. A.; et al. Optically Reconfigurable Chiral Microspheres of SelfOrganized Helical Superstructures with Handedness Inversion. Mater. Horizons 2017, 4 (6), 1190–1195.
Stumpel, J. E.; Broer, D. J.; Schenning, A. P. H. J. Stimuli-Responsive Photonic Polymer Coatings. Chem. Commun. 2014, 50 (100), 15839–15848.
Beltran-Gracia, E.; Parri, O. L. A New Twist on Cholesteric Films by Using Reactive Mesogen Particles. J. Mater. Chem. C 2015, 3 (43), 11335–11340.
Lee, S. S.; Kim, S. K.; Won, J. C.; Kim, Y. H.; Kim, S. H. Reconfigurable Photonic Capsules Containing Cholesteric Liquid Crystals with Planar Alignment. Angew. Chemie - Int. Ed. 2015, 54 (50), 15266–15270.
Noh, J.; Liang, H. L.; Drevensek-Olenik, I.; Lagerwall, J. P. F. Tuneable Multicoloured Patterns from Photonic Cross-Communication between Cholesteric Liquid Crystal Droplets. J. Mater. Chem. C 2014, 2 (5), 806–810.
Aßhoff, S. J.; Sukas, S.; Yamaguchi, T.; Hommersom, C. A.; Le Gac, S.; Katsonis, N. Superstructures of Chiral Nematic Microspheres as All-Optical Switchable Distributors of Light. Sci. Rep. 2015, 5, 1–10.
Wang, X.; Bukusoglu, E.; Abbott, N. L. A Practical Guide to the Preparation of Liquid CrystalTemplated Microparticles. Chem. Mater. 2017, 29 (1), 53–61.
Ko, S.-W.; Huang, S.-H.; Fuh, A. Y.-G.; Lin, T.-H. Measurement of Helical Twisting Power Based on Axially Symmetrical Photo-Aligned Dye-Doped Liquid Crystal Film. Opt. Express 2009, 17 (18), 566–571.
Bouligand, Y.; Livolant, F. The Organization of Cholesteric Spherulites. J. Phys. 1984, 45, 1899– 1923.